Biogenic synthesis and characterization of gold nanoparticles by Escherichia coli K12 and its heterogeneous catalysis in degradation of 4-nitrophenol
© Srivastava et al.; licensee Springer. 2013
Received: 28 November 2012
Accepted: 28 January 2013
Published: 12 February 2013
Room-temperature extracellular biosynthesis of gold nanoparticles (Au NPs) was achieved using Escherichia coli K12 cells without the addition of growth media, pH adjustments or inclusion of electron donors/stabilizing agents. The resulting nanoparticles were analysed by ultraviolet–visible (UV–vis) spectrophotometry, atomic force microscopy, transmission electron microscopy and X-ray diffraction. Highly dispersed gold nanoplates were achieved in the order of around 50 nm. Further, the underlying mechanism was found to be controlled by certain extracellular membrane-bound proteins, which was confirmed by Fourier transformation-infrared spectroscopy and sodium dodecyl sulfate polyacrylamide gel electrophoresis. We observed that certain membrane-bound peptides are responsible for reduction and subsequent stabilization of Au NPs (confirmed by zeta potential analysis). Upon de-activation of these proteins, no nanoparticle formation was observed. Also, we prepared a novel biocatalyst with Au NPs attached to the membrane-bound fraction of E. coli K12 cells serving as an efficient heterogeneous catalyst in complete reduction of 4-nitrophenol in the presence of NaBH4 which was studied with UV–vis spectroscopy. This is the first report on bacterial membrane-Au NP nanobiocomposite serving as an efficient heterogeneous catalyst in complete reduction of nitroaromatic pollutant in water.
KeywordsGold nanoparticles Extracellular biosynthesis Green catalysis Escherichia coli Nitrophenol degradation Water treatment
Gold nanoparticle (Au NP), being the most stable mono-metallic nanoparticle, promises to be a key material and building block for newer technologies in the twenty-first century. Gold in its bulk state is regarded as a noble metal and is very unreactive because of its completely filled d-band. However, at nanoscale, it is proving to be an important material for catalysis owing to its shape, size and crystal structure arrangement. Due to this new set of properties, it has found wide-scale application in optics, electronics, catalysis, fabrication and biomedical utilities. Generally speaking, physical methods of producing gold nanoparticles involve heating of gold at reduced pressure to generate gold vapour, while chemical synthesis requires a reducing agent (generally citrate) followed by addition of a stabilizing agent[4–7]. However, these chemical methods deliver at the cost of expensive reducing and capping agents and toxic solvents along with tedious process control. To overcome these issues, several biogenic synthesis processes have been reported owing to the constant need for cost-effective eco-friendly synthesis of Au NPs. Microbial systems have found an important role in nanoparticle production due to their natural mechanism for detoxification of metallic ions through reduction which can be achieved extracellularly or intracellularly through bioaccumulation, precipitation, biomineralization and biosorption. Ogi et al. showed gold nanoparticle formation in the presence of H2 gas pumped with Shewanella algae cell extract. Similarly, gold nanoparticles of different shapes and sizes were produced using bacterial and fungal strains[9–12]. However, apart from the stated advantages, biological synthesis suffers from poor mono-dispersity, random aggregation, non-uniform shapes, problems in scale-up, etc.. Though, in recent times, many organisms have been reported to produce nanoparticles, scientific understanding on the mechanism and the machinery related to its production is still in its infancy. Therefore, there is a need to improve upon this green synthesis process with an aim to understand the underlying mechanism and design a working prototype for biomimetic production of Au NPs.
These nanoparticles, upon being adhered to a matrix, may serve as a better catalyst than bulk metal due to greater accessibility to surface atoms and low coordination number especially in the case of water treatment. Among several water pollutants, nitroaromatic compounds are considered as the most toxic and refractory pollutants, of which the permissible range is as low as 1 to 20 ppb. However, these are common in production of dyes, explosives and pesticides among many others; thus, their industrial production is considered as an environmental hazard. Upon being released into the environment, these nitrophenols pose significant public health issues by exhibiting carcinogenic and mutagenic potential in humans.
Normally, it takes a long time for degradation of nitrophenols in water which poses considerable risk if it seeps into aquifers along with the groundwater. These nitrophenols tend to get accumulated in deep soil and stays indefinitely. Although several water treatment methods are available like chemical precipitation, ion exchange adsorption, filtration and membrane systems, they are slow and non-destructive. Therefore, there is a need to remove these highly toxic compounds with efficient catalytic systems. Generally, nanoparticles are immobilized onto supporting materials like silica, zeolites, resins, alumina, microgels, latex, etc. which are inert to the reactants and provide a rigid framework to the nanoparticles. The gold-supported catalysts can then be used to carry out partial or complete oxidation of hydrocarbons, carbon monoxide, nitric oxide, etc.. In a recent study, Deplanche et al. showed coating of palladium followed by gold over Escherichia coli surface in the presence of H2 to produce biomass-supported Au-Pd core-shell-type structures and subsequent oxidation of benzyl alcohol. Likewise, we believe that bacterial biomass is essentially carbonaceous matter which can be used to serve as a matrix for preparing a heterogeneous catalyst with the incorporation of nanoparticles. With this aim, we utilized E. coli K12 strain to check its potential for producing Au0 from AuCl4 −. This strain has been known for its reduction activity as shown with bioremediation studies[18, 19]. Here, we report bioreduction of gold cations at room temperature to yield well-dispersed nanoparticles (Au0). The resulting nanoparticles were characterized by ultraviolet–visible (UV–vis) spectroscopy, atomic force microscopy (AFM), selected-area electron diffraction (SAED), transmission electron microscopy (TEM) and X-ray diffraction (XRD). Additionally, the extracellular reduction mechanism was examined by Fourier transformation-infrared spectroscopy (FT-IR), zeta potential (Z-pot) and sodium dodecyl sulfate polyacrylamide gel electrophoresis (SDS-PAGE). We observed that certain membrane-embedded proteins in the extracellular membrane fraction of the cell are responsible for reducing gold cation to stable Au0 state. Further, these membrane-bound gold nanoparticles were utilized to produce a heterogeneous catalyst in degradation of 4-nitrophenol (4-NP). This biosynthesis study provides an excellent platform for the production of gold nanoparticles by bacterial membrane-bound proteins. The resulting membrane-bound nanoparticles can be prepared into an eco-friendly cost-effective bionanocomposite to serve as an efficient catalyst in complete degradation of 4-nitrophenol.
Bacterial strain and growth conditions
E. coli K12 cells were procured from our existing strain collection and were cultured in nutrient broth (10 g L−1 peptone, 10 g L−1 meat extract, 0.5 g L−1 NaCl) at 27°C and 120 rpm for 24 h in screw-capped flasks. After a day of incubation, the culture was centrifuged at 10,000×g for 10 min, and the resulting bacterial pellet was separated and retained. The bacterial pellet was thoroughly washed three times in sodium saline followed by washing three times in Milli-Q water (Millipore, Tokyo, Japan) to remove any unwanted material sticking to the cells. These cells were weighed, and 0.5 g wet weight of pellet was prepared to be used later. The washed cells suspended in 10 mL of distilled water gave a solution with a cell concentration of 5.2 × 1011 cells mL−1.
To determine whether or not intact cells were required for Au NP formation, E. coli K12 cells were cultured and harvested as in the previously described method. The cells were then disrupted by autoclaving (120°C at 15 psi for 30 min). This caused complete lysis of the bacterial cells which were later centrifuged at 15,000×g for 60 min to separate the membrane fraction (pellet) from the soluble (supernatant) fraction. Membrane-bound fraction (MBF) pellet was pooled together and washed thrice with Milli-Q water and re-centrifuged again at 15,000×g for 30 min. Finally, 2 g of MBF pellet (wet wt.) was retained to be incorporated with 10 mL of 0.01 M HAuCl4 solution (Nacalai Tesque, Kyoto, Japan). Although pH was measured at this stage (pH 2.8), no adjustment was made. Control reactions included 0.01 M HAuCl4 solution prepared with soluble (supernatant) fraction and uninoculated HAuCl4 solution prepared with Milli-Q water.
Characterization of biogenic gold nanoparticles
UV-visible spectra were obtained using a Hitachi U2000A UV–vis spectrophotometer (Tokyo, Japan). The formation of Au NPs was monitored by UV–vis spectra of the reaction mixture from 210 to 800 nm.
Primary study of nanoparticle shape and size was carried out using an SPI-3800N atomic force microscope with SPA 400 soundproof housing sample holder connected to an imaging system (Seiko Instruments, Chiba, Japan). Five microlitres was taken from the reaction mixture and placed on the glass grid and dried at room temperature. The images were obtained using SPIWin (3800N) ver. 3.02J (Wyandotte, MI, USA).
Morphology and grain size of these nanoparticles were analysed using a Hitachi H-7100 transmission electron microscope. Two microlitres was taken from the two reaction mixtures and placed on carbon-coated copper grids and dried at room temperature. The transmission electron micrographs and the SAED patterns were recorded at an acceleration voltage of 100 kV. The images were analysed using the ImageJ 1.43M software.
FT-IR analysis was done using Jasco FT/IR-680 plus (Easton, MD, USA) coupled to a high-performance computer. The samples (100 μL) were placed over the ATR analyser, and the resulting spectra were analysed using Spectra Manager ver. 1.06.02. Zeta potential measurements were performed using the Malvern Zetasizer Nano ZS model ZEN3600 (Malvern, UK) equipped with a standard 633-nm laser.
Confirmatory study of resulting Au NPs was done by XRD using a Rigaku RINT-TTR diffractometer (Tokyo, Japan) equipped with a parallel incident beam (Göbel mirror) and a vertical θ-θ goniometer. Samples were placed directly on the sample holder. The X-ray diffractometer was operated at 50 kV and 300 mA to generate CuKα radiation. The scan rate was set to 5° mil−1. Identification of the metallic gold was obtained from the JCPDS database.
Preparation of biomass-supported Au nanocatalyst in 4-nitrophenol degradation
The reduction of 4-NP by NaBH4 was studied as a model reaction to probe catalytic efficiency of a biomass-supported Au catalyst for heterogeneous systems. Under experimental conditions, reduction does not proceed at all simply with the addition of NaBH4 or biomass alone. However, in the presence of a biomass-supported Au catalyst, it proceeds to completion with formation of 4-aminophenol (4-AP). To study the reaction in a quartz cuvette, 2.77 mL of water was mixed with 30 μL (10−2 M) of 4-NP solution and 200 μL of freshly prepared NaBH4 (10−1 M) was added. The Au NP reaction mixture along with the MBF was dried for 24 h at 90°C, and 5 mg of biomass-Au NP composite (size approximately 50 nm, 4.2 × 10−6 mol dm−3) was added to the above reaction mixture. A similar technique was used by Narayanan and Sakthivel by coating fungal mycelia-coated Au NPs on glass beads. UV–vis spectra of the sample were recorded at every 2-min interval in the range of 200 to 600 nm. The rate constant of the reduction process was determined by measuring the change in absorbance of the initially observed peak at 400 nm, for the nitrophelate ion as the function of time.
Results and discussion
Characterization of biogenic Au NPs
FT-IR spectra (Figure 3a) confirmed the presence of vibration bands centred at 1,841, 1,787, 1,756, 1,725, 1,692, 1,680, 1,661, 1,650, 1,634 and 1,603 cm−1. This highlights the presence of amide I (C=O) and amide II (N=H) groups present in the reaction mixture. It is likely that the amide carbonyl group (C=O) arises from peptide coupling in proteins from the extracellular membrane fraction of the bacterial cell. This supports the fact that the secondary amide C=O stretching which forms protein/Au bioconjugates may have a role in stabilization of nanoparticles. Generally, in the case of biogenic synthesis, the presence of active chemical groups like amino, sulfhydryl and carboxylic groups plays a key role in reduction of metallic ions and subsequent formation of nano/microparticles. Since amino and carboxyl groups were detected by FT-IR, it strongly suggested towards the presence of certain proteins in the reaction medium responsible for Au NP biosynthesis. Further, aqueous stability of Au NPs were tested by zeta potential analysis. It should be noted that if active groups on biomass carry greater positive charge at low pH, it weakens the reducing power of biomass and allows AuCl4 − ions to get closer to the reaction site. This decreases the reaction rate and causes strong biosorption between Au NPs and biomass resulting in particle aggregation. Since the bacterial cell wall of E. coli is negatively charged, it tends to thermodynamically favour the formation of nanoparticles at low pH as observed in our case. This was confirmed by zeta potential analysis of the Au NP solution with a mean Z-pot of −24.5 ± 3.1 mV, suggesting a stable gold colloid solution. To further investigate the role of proteins in nanoparticle formation, MBF was treated with 1% β-mercaptoethanol (β-met) and heated for 30 min at 95°C. This treatment caused disruption of disulfide bonds within the multimeric chains of peptide and eventually resulted in loss of activity. In the absence of reducing activity by membrane-bound proteins, no nanoparticle formation was observed with β-met-treated MBF. This was further verified by FT-IR analysis (Figure 3b) with disappearance of most bands around the 1,600 cm−1 region. The peak observed at 1,075 cm−1 corresponds to the thiocarbonyl group due to the addition of mercaptoethanol in the reaction mixture. This suggested that certain membrane-embedded proteins may be responsible for reducing Au3+ to Au nanoparticles (Au0). The membrane proteins responsible for nanoparticle synthesis were run along with β-met-treated membrane proteins in SDS-PAGE gel (data not shown) which confirmed the presence of different sizes of protein bands in the reaction mixture, of which 25 and 73 KDa seemed to be of importance. Upon treatment of MBF with β-met, there was absence of a protein band at 73 KDa, and subsequently, no nanoparticle formation was observed, suggesting its crucial role in the reduction process. Also, a shorter peptide (25 KDa) was found to be adhered to the synthesized nanoparticles, suggesting its role in stabilization of nanoparticles. This is in accordance with our recently reported study where we concluded that ionic reduction in some bacteria takes place due to certain proteins along the lipopolysaccharides/cell wall which reduces the metallic ions in its vicinity of the bacterial cell, thereby producing stable nanoparticles.
Catalytic activity of Au-MBF biocatalyst in 4-nitrophenol degradation
Aqueous 4-NP shows maximum UV–vis absorbance at 317 nm. When NaBH4 (pH > 12) was added to reduce 4-NP, an intense yellow colour appeared due to formation of 4-nitrophenolate ion red-shifting the absorption peak to 400 nm. The reaction does not proceed, and the peak remained for several days in the absence of Au catalyst[28, 29]. Also, no peak change was observed in the control reaction consisting of MBF only without Au NPs.
Extracellular membrane fraction of E. coli K12 was found to be responsible for the biogenic synthesis of gold nanoparticles at room temperature without pH adjustment. Gold nanoplates were obtained in majority in the size range of around 50 nm. We concluded that certain proteins embedded in the membrane fraction cause formation and stabilization of Au NPs. In the absence of these proteins (activity loss by β-met treatment), no nanoparticle formation was observed. Since biogenic nanoparticles are stabilized ‘naturally’ in the presence of active biomass, their efficacy in the preparation of heterogeneous catalyst was examined. We provided an innovative approach to utilize biogenic gold nanoparticles adsorbed over the cell membrane fraction to be used as a heterogeneous catalyst for catalysing complete degradation of 4-NP. A distinct advantage of this study lies in the fact that the facile green synthesis process can be seamlessly aligned with the preparation of nanobiocatalyst which may find numerous applications in catalysis, bioremediation studies, etc. This research has the potential to promote membrane fractions (proteins) for continuous synthesis of different types of NPs (see Additional file1) and subsequent development of associated bionanocomposite resulting in improved material synthesis and application by biogenic systems.
This work was partly supported by the Special Coordination Fund for Promoting Science and Technology, Creation of Innovative Centers for Advanced Interdisciplinary Research Areas (Innovative BioProduction Kobe) from the Ministry of Education, Culture, Sports and Technology (MEXT) and by the MEXT Scholarship research fund. We also extend our sincere gratitude to Dr. Yasukiyo Ueda for his assistance with TEM observations, Dr. Atsunori Mori for his assistance with FT-IR and Dr. Yuzuru Mizuhata for his assistance with XRD. SKS would like to thank Ms. Charu Srivastava (TCS, India) for her constant support and insightful discussions leading to the completion of this research.
- Bond GC, Thompson DT: Catalysis by gold. Catal Rev Sci Eng 1995, 41: 319–388.View Article
- Narayanan R, El-Sayed MA: Catalysis with transition metal nanoparticles in colloidal solution: nanoparticle shape dependence and stability. J Phys Chem B 2005, 109: 12663–12676. 10.1021/jp051066pView Article
- Daniel MC, Astruc D: Gold nanoparticles: assembly, supramolecular chemistry, quantum-size-related properties and applications toward biology, catalysis, and nanotechnology. Chem Rev 2004, 104: 293–346. 10.1021/cr030698+View Article
- Murphy CJ, Sau TK, Gole AM, Orendorff CJG, Gou JL, Hunyadi SE, Li T: Anisotropic metal nanoparticles: synthesis, assembly, and optical applications. J Phys Chem B 2005, 109: 13857–13870. 10.1021/jp0516846View Article
- Pileni MP: The role of soft colloidal templates in controlling the size and shape of inorganic nanocrystals. Nat Mater 2003, 2: 145–149. 10.1038/nmat817View Article
- Brust M, Kiely CJ: Some recent advances in nanostructure preparation from gold and silver particles: a short topical review. Colloid Surface A 2002, 202: 175–186. 10.1016/S0927-7757(01)01087-1View Article
- Genc R, Clergeaud G, Ortiz M, O’Sullivan CK: Green synthesis of gold nanoparticles using glycerol-incorporated nanosized liposomes. Langmuir 2011, 27: 10894–10900. 10.1021/la201771sView Article
- Ogi T, Saitoh N, Nomura T, Konishi Y: Room-temperature synthesis of gold nanoparticles and nanoplates using Shewanella algae cell extract. J Nanopart Res 2010, 12: 2531–2539. 10.1007/s11051-009-9822-8View Article
- Nair B, Pradeep T: Coalescence of nanoclusters and formation of submicron crystallites assisted by Lactobacillus strains. Cryst Growth Des 2002, 2: 293–298. 10.1021/cg0255164View Article
- Gericke M, Pinches A: Microbial production of gold nanoparticles. Gold Bull 2006, 39: 22–28. 10.1007/BF03215529View Article
- Das SK, Das AR, Guha AK: Gold nanoparticles: microbial synthesis and application in water hygiene management. Langmuir 2009, 25: 8192–8199. 10.1021/la900585pView Article
- Thakkar KN, Mhatre SS, Parikh RY: Biological synthesis of metallic nanoparticles. Nanomed-Nanotechnol 2010, 6: 257–262. 10.1016/j.nano.2009.07.002View Article
- Narayanan KB, Sakthivel N: Biological synthesis of metal nanoparticles by microbes. Adv Colloid Interface Sci 2010, 156: 1–13. 10.1016/j.cis.2010.02.001View Article
- Booth G: Nitro Compounds, Aromatic in Ullmann’s Encyclopedia of Industrial Chemistry. New York: Wiley; 2007.
- Pohanish RP: Sittig’s Handbook of Toxic and Hazardous Chemicals and Carcinogens. Amsterdam: Elsevier; 2011.
- Haruta M: Size and support dependency in the catalysis of gold. ChemInform 1997, 28: 153–166.
- Deplanche K, Merroun ML, Casadesus M, Tran DT, Mikheenko IP, Bennett JA, Zhu J, Jones IP, Attard GA, Wood J, Selenska-Pobell S, Macaskie LE: Microbial synthesis of core/shell gold/palladium nanoparticles for applications in green chemistry. J R Soc Interface 2012, 9: 1705–1712. 10.1098/rsif.2012.0003View Article
- Pazirandeh M, Wells BM, Ryan RL: Development of bacterium-based heavy metal biosorbents: enhanced uptake of cadmium and mercury by Escherichia coli expressing a metal binding motif. Appl Environ Microbiol 1998, 64: 4068–4072.
- Ackerley DF, Barak Y, Lynch SV, Curtin J, Matin A: Effect of chromate stress on Escherichia coli K-12. J Bacteriol 2006, 188: 3371–3381. 10.1128/JB.188.9.3371-3381.2006View Article
- Narayanan KB, Sakthivel N: Synthesis and characterization of nano-gold composite using Cylindrocladium floridanum and its heterogeneous catalysis in the degradation of 4-nitrophenol. J Hazard Mater 2011, 189: 519–525. 10.1016/j.jhazmat.2011.02.069View Article
- Link S, El-Sayed MA: Shape and size dependence of radiative, nonradiative, and photothermal properties of gold nanocrystals. Int Rev Phys Chem 2000, 19: 409–453. 10.1080/01442350050034180View Article
- Basu S, Panigrahi S, Praharaj S, Ghosh SK, Pande S, Jana S, Pal T: Dipole–dipole plasmon interactions in self-assembly of gold organosol induced by glutathione. New J Chem 2006, 30: 1333–1339. 10.1039/b607399aView Article
- Gole A, Dash C, Ramachandran V, Mandale AB, Sainkar SR, Mandale AB, Rao M, Sastry M: Pepsin−gold colloid conjugates: preparation, characterization and enzymatic activity. Langmuir 2001, 17: 1674–1679. 10.1021/la001164wView Article
- He S, Guo Z, Zhang Y, Zhang S, Wang J, Gu N: Biosynthesis of gold nanoparticles using the bacteria Rhodopseudomonas capsulate. Mater Lett 2007, 61: 3984–3987. 10.1016/j.matlet.2007.01.018View Article
- Srivastava SK, Constanti M: Room temperature biogenic synthesis of multiple nanoparticles (Ag, Pd, Fe, Rh, Ni, Ru, Pt, Co, and Li) by Pseudomonas aeruginosa SM1. J Nanopart Res 2012, 14: 831.View Article
- Pradhan N, Pal A, Pal T: Catalytic reduction of aromatic nitro compounds by coinage metal nanoparticles. Langmuir 2001, 17: 1800–1802. 10.1021/la000862dView Article
- Ghosh SK, Mandal M, Kundu S, Nath S, Pal T: Bimetallic Pt–Ni nanoparticles can catalyze reduction of aromatic nitro compounds by sodium borohydride in aqueous solution. Appl Catala-Gen 2004, 268: 61–66. 10.1016/j.apcata.2004.03.017View Article
- Hayakawa K, Yoshimura T, Esumi K: Preparation of gold−dendrimer nanocomposites by laser irradiation and their catalytic reduction of 4-nitrophenol. Langmuir 2003, 19: 5517–5521. 10.1021/la034339lView Article
- Lu Y, Mei Y, Ballauff M: Thermosensitive core−shell particles as carrier systems for metallic nanoparticles. J Phys Chem B 2006, 110: 3930–3937. 10.1021/jp057149nView Article
- Pradhan N, Palb A, Pal T: Silver nanoparticle catalyzed reduction of aromatic nitro compounds. Colloid Surface A 2002, 196: 247–257. 10.1016/S0927-7757(01)01040-8View Article
- Scott RWJ, Wilson OM, Crooks RM: Synthesis, characterization and applications of dendrimer-encapsulated nanoparticles. J Phys Chem B 2005, 109: 692–704. 10.1021/jp0469665View Article
- Panigrahi S, Basu S, Praharaj S, Pande S, Jana S, Pal A, Ghosh SK, Pal T: Synthesis and size-selective catalysis by supported gold nanoparticles: study on heterogeneous and homogeneous catalytic process. J Phys Chem C 2007, 111: 4596–460.View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.